doi: 10.1111/ffe.12578

Fatigue crack closure: a review of the physical phenomena R. PIPPAN1 and A. HOHENWARTER2 1

Erich Schmid Institute of Materials Science, Austrian Academy of Sciences, Leoben 8700, Austria, 2Department of Materials Physics, Montanuniversität Leoben, Leoben 8700, Austria Received Date: 12 October 2016; Accepted Date: 21 December 2016; Published Online: 1 February 2017

A B S T R A C T Plasticity-induced, roughness-induced and oxide-induced crack closures are reviewed.

Special attention is devoted to the physical origin, the consequences for the experimental determination and the prediction of the effective crack driving force for fatigue crack propagation. Plasticity-induced crack closure under plane stress and plane strain conditions require, in principle, a different explanation; however, both types are predictable. This is even the case in the transition region from the plane strain to the plane stress state and all types of loading conditions including constant and variable amplitude loading, the short crack case or the transition from small-scale to large-scale yielding. In contrast, the prediction of roughness-induced and oxide-induced closures is not as straightforward. Keywords fatigue crack growth; oxide-induced crack closure; plasticity-induced crack closure; roughness-induced crack closure; threshold.

NOMENCLATURE

ΔCTOD Δrpl dn ui d ΔKeff Δσ eff or Δεeff εy Δε n b xmin rpl xi α Κmax Kmin K ΔK Kcl Kop R ΔKeff,th σy E

= = = = = = = = = = = = = = = = = = = = = = = = =

cyclic crack tip opening displacement cyclic plastic zone size dimensionless factor describing hardening behaviour and stress state displacements into the principal directions with i = 1,2,3 distance between dislocations effective stress intensity range effective stress or strain range elastic strain contribution entire strain range hardening exponent magnitude of burgers vector minimum width of a wedge monotonic plastic zone size principal directions with i = 1,2,3 rotation angle stress intensity at maximum load stress intensity at minimum load stress intensity factor stress intensity factor range stress intensity factor when ﬁrst contact between crack ﬂanks occurs stress intensity factor when last crack ﬂank contact opens stress ratio (=Kmin/Kmax) threshold of effective stress intensity factor range yield stress Young’s modulus

Correspondence: A. Hohenwarter. E-mail: [email protected]

This is an open access article under the terms of the Creative Commons Attribution License, which permits use, distribution and reproduction in any medium, provided the original work is properly cited. © 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

471

472

R. PIPPAN AND A. HOHENWARTER

INTRODUCTION

In order to understand the fatigue crack propagation behaviour of materials as a function of loading condition, for instance, stress or strain amplitude, stress ratio, load history, environment, mixed mode loading, large-scale or small-scale yieldings and so on, it is very helpful to separate the different mechanisms affecting the crack propagation rate into intrinsic and extrinsic mechanisms.1 The intrinsic mechanisms cause the formation of new fracture surfaces at the crack tip. They are controlled by the monotonic and cyclic strains applied to the volume elements at and in front of the crack tip. For cyclic loading signiﬁcantly below the fracture toughness, the cyclic deformation is the dominant part responsible for fatigue crack propagation. In fatigue of ductile metals, the crack extension per cycle is usually caused by plastic blunting and re-sharpening of the crack tip,2–10 except for loads near the fracture toughness where static fracture or monotonically induced damage ahead of the crack tip can contribute signiﬁcantly to the crack extension in each cycle. The contribution of monotonic loading-induced fracture is more important in brittle materials such as intermetallic alloys, ceramics and some cast alloys. The extrinsic mechanisms affect the monotonic and cyclic deformation at the crack tip and as a consequence inﬂuence the crack growth rate. The mechanisms that decrease or increase the deformation can have a shielding or anti-shielding effect, respectively. Ritchie1 and Suresh11 classiﬁed the different extrinsic mechanisms into geometric, zone and contact shielding mechanisms and combined zone and contact shielding mechanisms. The geometric mechanisms, such as crack deﬂection or branching, are a consequence of the deviation of the real crack shape from the ideal plane crack with a straight crack front. They induce a local variation of the stress and strain ﬁelds at the crack along the crack front during crack propagation, which can be expressed by a local variation of the crack driving force and a mixing of the local loading modes. The zone shielding effects, for example, phase transformation, plasticity or residual stresses, also change the stress and strain ﬁelds, but can induce fracture surface contact during cyclic loading as well, similar to the other contact mechanisms. The essence of the contact shielding mechanisms is a load transfer between the crack faces reducing the monotonic as well as the cyclic deformation at the crack tip during one load cycle compared with cracks where such load transfer is not active. Therefore, contact shielding mechanisms by corrosion debris-induced closure (often denoted as oxide-induced crack closure), roughnessinduced closure, crack bridging by ligaments or ﬁbres, sliding crack surface interference and the combined zone

and contact shielding mechanisms by plasticity-induced crack closure and phase transformation-induced crack closure are essential for the understanding of the fatigue crack propagation phenomena. Crack bridging by ligaments and ﬁbres is important especially in brittle materials and composites, respectively,12–18 whereas sliding crack surface interference is more important under mixed mode loading.1,19 These two mechanisms can induce a load transfer during the whole load amplitude, therefore reducing the monotonic and the cyclic deformation of the crack tip. On the other hand, crack closure induced by plasticity, roughness and corrosion debris causes a load transfer only during a certain part near the minimum load of the load amplitude and therefore only affects the cyclic deformation of the crack tip. In order to make the consideration easier, the present paper focuses only on the effect of these closure mechanisms. Despite the vast number of papers dealing with these mechanisms and their origin, the measurability and predictability, as well as their dependence on loading history, microstructure or crack length, there are several essential discrepancies regarding their interpretation and importance in the fatigue community. The present paper is not thought to be a summary of about 10 000 papers dealing with this subject but is more intended to be a critical review dealing with the origin of crack closure, the measurability and predictability of the closure itself as well as its importance in lifetime simulation and the open questions in the different areas. It should be pointed out that this review concentrates on the phenomena of crack closure exclusively for external Mode I loading, because for Modes II and III, the sliding contacts (which reduce strongly the effective driving force) act during the whole load amplitude and the driving force cannot be simply determined by KmaxKCl. The paper will start with a short historical overview, drawing then special attention to the physical origin of the fracture surface contacts in the tensile part of the loading, moving to the effect of contact forces on the crack stress ﬁeld and discussing shortly the measurability, the predictability and the important parameters affecting crack closure under small-scale yielding condition. Finally, the effect of closure under large-scale or full-scale yielding, which is typical for low cycle fatigue, will be considered. Historical background The ﬁrst observations on early crack initiation and the following fatigue crack propagation during cyclic loading were published by Ewing and Humphrey.20,21 For a long time, fatigue crack growth investigations had been performed solely by optical microscopes. The development of the electron microscopes in the 1950s

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

FATIGUE CRACK CLOSURE

helped to discover special features such as striations, which indicate the cycle per cycle nature of crack growth.22 The application of the fracture mechanics started with the use of the stress intensity factor range to describe fatigue crack propagation by Paris23 in the beginning of the 1960s. Rice introduced a simple transformation scheme24 and suggested that the cyclic deformation in front of a crack could be described by the same equations as in the case of monotonic loading. One has only to exchange the stress intensity factor K by the stress intensity factor range ΔK = KmaxKmin, and the yield stress becomes twice the monotonic yield stress. Hence, the cyclic plastic zone, the cyclic plastic strain in front of the crack tip and the cyclic crack tip opening displacement is only a function of the ΔK and the cyclic plastic properties of the material. At the same time, the ﬁrst damage24 and geometrical deformation models2–5 were proposed to explain the fatigue crack propagation behaviour. In 1970, Elber25,26 discovered that a contact between the fracture surfaces could take place even during cyclic tensile loading. He attributed the occurrence of this fracture surface contact to the plastic deformation in the wake of a growing crack. This mechanism is nowadays usually called plasticity-induced crack closure. During the following decade, several other mechanisms responsible for premature contact of the fracture surface were proposed: roughness-induced crack closure,27–31 oxideinduced crack closure or often termed corrosion and phase debris-induced crack closure32–37 transformation-induced crack closure.37–39 A further important ﬁnding in the 1970s was the so-called short crack effect,40–43 which means that at the same driving force, ΔK, short cracks grow faster than long cracks, and short cracks can propagate even below the ΔKth of a long crack. In the 1980s, it was shown that it was very helpful to subdivide the short crack phenomena into different types of short cracks, namely, microstructurally short, mechanically short, physically short and chemically short cracks.11,41 Most of the studies in the last four decades used the crack closure effect as a key to understand the effects of load ratio and load interaction, the behaviour of physically short cracks and many of the microstructural effects on fatigue crack propagation. Despite the huge number of studies supporting the importance of crack closure, there are several papers that noticed doubts on this concept; see, for example, Refs. [37, 44, 45]. In particular, plasticity-induced crack closure under plane strain loading conditions has been mistrusted, along with roughness-induced and debris-induced crack closures. The criticisms were most clearly pointed out in a paper of Louat et al. with the following statement44:

473

Plasticity originating from the crack tip does not induce crack closure and closure arising from asperity ridges due to oxides, corrosion products or surface roughness is small and insigniﬁcant unless the crack is completely packed with asperities. Despite some intense discussions45–49 and attempts of clariﬁcation,50–54 some discrepancies regarding the importance of crack closure seem to be unsolved. The basic questions are as follows: • Can da/dN be described solely by ΔKeff (or another effective driving force, for example, ΔJeff) and • Can ΔKeff be simply calculated by ΔK eff ¼ K max K cl

(1)

where Kmax is the maximum of the stress intensity factor and Kcl is the stress intensity factor where the ﬁrst fracture surface contact takes place. This review will try to shed light onto some of these discrepancies and will point out a few important open questions.

CLOSURE MECHANISMS

In this chapter, the physical origin of plasticity-induced, roughness-induced and oxide-induced crack closures will be discussed. As mentioned in the Introduction, they are especially important in ductile materials. Ligament and ﬁbre bridging as well as sliding crack surface interference will not be considered here. In the latter case, ΔKeff can deﬁnitely not be determined by Eq. (1), because there exists no deﬁned Kcl. For the determination of the effective ΔK, the load transfer between the crack ﬂanks at Kmin and Kmax would have to be known. In this case, a possible method to determine experimentally the effective ΔK would be given by an accurate analysis of the near crack tip opening displacement.13 Because of the 3D shape of the crack, and when additionally plasticity is involved, this analysis can be quite difﬁcult and is not in focus of this paper. Plasticity-induced crack closure For the explanation of the plasticity-induced crack closure, one has to distinguish between plane strain and plane stress case. For the plasticity-induced crack closure under plane stress condition, the explanation is simple, and it is well accepted in the fatigue community. Under plane stress conditions, the volume elements in the plastic zone are elongated. This elongation is mainly balanced by an out of the plane ﬂow of the material – that is, the thickness within the plastic zone is reduced, as

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

474

R. PIPPAN AND A. HOHENWARTER

Fig. 1 Illustration of the origin of the plasticity-induced crack closure under plane stress conditions. The out-of-plane ﬂow of the material in the plastic zone induces an elongation of the volume elements. The effect of the plastic wake on the cyclic plastic deformation can be interpreted as a wedge ﬁlled into the crack. [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

schematically illustrated in Fig. 1. When the crack propagates through the plastic zone, the stretched plastic wake comes into contact in the tension phase of the load amplitude. Hence, the plasticity-induced crack closure under plane stress conditions can be expressed as a consequence of an extra material layer behind the crack tip, which can be considered as a wedge that is inserted in the crack and reduces the cyclic plastic deformation at the crack tip and hence the fatigue crack growth rate. The formation of this plastic wedge is properly described by the Dugdale55 model worked out by Budiansky and Hutchinson,56 Führing and Seeger57 and by the mostly used modiﬁed versions of Newman.58 These strip yield models are well established to describe the stress ratio effects, load interaction effects or short crack effects.59–61 However, the disadvantage is that these models can only describe physically correct closure for the plane stress case. Newman62 tried to reﬂect the plane strain case with some adaptions. The situation for the plasticity-induced crack closure under plane strain condition is signiﬁcantly different. The crucial point is that there seems to be no source for the plastic wedge, because out-of-plane ﬂow is by deﬁnition not possible. This point has been clearly expressed by McEvily.63 ‘Suppose a crack is growing at a constant load and that the plasticity induced crack closure is occurring in the wake of the crack tip. This closure requires that more material will be behind the tip than it was there before. If the crack grows over some distance, say one meter, where does all the extra material in the wake of the crack

come from now?’ For a crack grown over a distance signiﬁcantly larger than the size of the plastic zone under plane strain conditions with constant stress intensity range or constant load, ε33, ε11 and as consequence ε22 should be 0 in the wake of the crack tip if the volume during plastic deformation remains constant, which is assumed in all analytical or numerical analyses. In reality, the plasticity of metals and alloys generates dislocations and vacancies. The vacancies induce a volume increase as well as dislocations. The latter is an effect of the nonlinearity in the near core dislocation stress ﬁeld and the core itself. However, the effect of volume increase due to plastic deformation is small; even in severely plastically deformed metals, the increase is only in the order of 104 as shown recently.64 Therefore, the question remains where does the extra material come from? Under plane strain conditions and a constant ΔK or constant load amplitudes, there is no plastic wedge at large distances behind the crack tip. However, the material in the plastic wake is plastically deformed. It is plastically sheared; this shearing induces a rotation of the volume elements, and as a consequence, a local wedge is formed in the vicinity of the crack tip.50,51,54 There are different ways to visualize this material transfer to the crack tip due to imbedded plastic deformation in the elastic surrounding. For material scientists, the description by geometrically necessary dislocations is the simplest one50 (Fig. 2a). Here, the rotation of the volume elements is induced by the ‘small angle grain boundary-like’ arrangement of the geometrically necessary dislocations in the plastic wake (Fig. 2a & b). From a continuum mechanic point of view (Fig. 2c & d), the constraint shear deformation can explain this material transport to the crack tip.51 Another explanation can be given by dislocation shielding considerations.46,54,65 Recently, this transfer from the plastic wake to the crack tip has been shown also by a ﬁnite element simulation.66,67 Figure 3 illustrates schematically the essential difference between the plane stress case (Fig. 3b), where the dominant effect is the elongation of the volume elements in the plastic wake,67 whereas in the plane strain case (Fig. 3a), only a local plastic wedge is formed near the crack tip with a length comparable with the size of the plastic zone.53 To make the differences clearer in Fig. 3, the ligament of the growing crack containing body is cut along the plane of the crack. As clearly evident from this illustration under plane strain condition, only local wedges or humps on the crack ﬂanks occur, which results from the transfer of the material in the crack propagation direction, for constant and for variable amplitudes, respectively.

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

FATIGUE CRACK CLOSURE

475

Fig. 2 Illustration of the effect of the plastic wake under plane strain and small-scale yielding conditions on a growing fatigue crack loaded under constant ΔK. (a) The plastic shear deformation induces a material transport to the crack tip shown as a consequence of geometrically necessary dislocations in the crack wake. (b) The rotation of the volume elements is visualized from the dislocation point of view: to realize the shear deformation, the geometrically necessary dislocations are arranged for simplicity in a single band and induce the lattice rotation.59 (c) Rotational transport of the material from continuum mechanics point of view for a single volume element and (d) for an arrangement of volume elements forming a growing crack.51 The shear deformation opens the crack, and without an elastic constraint, this shear deformation would result in a continuous increase of the crack opening displacement with increasing distance from the crack tip. In the unloaded case, the elastic constraint reduces the crack tip opening at lager distances from the crack tip to zero, causes a rotation of the volume elements and closing of the crack in the vicinity of the crack tip. [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

Fig. 3 Schematic illustrations of the effect of the plastic deformation of a growing crack illustrated for one specimen half. The resulting displacements are enlarged compared with the size of the plastic zone. (a) Displacement ﬁeld and the remaining contour, under plane strain conditions; at larger distances from the crack tip, the rotation induced from the shear deformation remains, only near the crack tip a hump is formed with an extension of the size of the monotonic plastic zone. (b) Displacement ﬁeld and the resulting contour in the plane stress case. Here, the elongation of the volume elements in the plastic wake form a wedge with a constant thickness, even a small effect of shearing takes place (for details, see Ref. [67]). The effect of an overload on the ‘crack’ contour in the case of an overload is depicted for the plane strain (c) and the plane stress (d) cases. [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

Roughness-induced crack closure The contact of the fracture surfaces caused by the misﬁt of the microscopically rough fracture surfaces is denoted as

roughness-induced crack closure. It was ﬁrst proposed in the early 1980s.27–31 The usual explanation of roughnessinduced crack closure is sketched in Fig. 4. At a macroscopic mode I loading, because of microstructural

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

476

R. PIPPAN AND A. HOHENWARTER

Fig. 4 Schematic illustration of roughness-induced crack closure due to a residual Mode II or Mode III displacement of rough fracture surfaces. The closure stress intensity is determined by the residual displacements u1 and u3, the geometry parameters of the rough fracture surfaces and the distance between the crack tip and the contact.

anisotropy and inhomogeneity, a local Modes II or III deformation takes place; this results in a local displacement in the crack propagation direction Δu1 or out of plane displacement Δu3. In polycrystalline materials, the local Modes II and III deformation vary along the fatigue crack front. In one grain, Δu1 and Δu3 can be positive, whereas in the neighbouring grains or even in the same grain nearby, an opposite displacement might occur. Hence, this mixed mode-induced displacement should be only a local phenomenon, because at larger distances behind the crack tip, the residual displacements from the different local crack tip deformation should cancel them out. However, from experimental studies,68 it is known that roughness-induced crack closure can build up over quite large distances, implying that there must be also a far-ﬁeld contribution to this closure type. It has been shown that the asymmetry in the deformation at the crack tip generates a misﬁt of rough fracture surfaces even far away from the crack tip.69 The explanation used earlier for the plasticity-induced crack closure under plane strain condition can be simply adapted to explain the roughness-induced crack closure. The plasticity-induced crack closure is explained by a transfer of material to the crack tip; this transfer can be expressed by a displacement of the crack ﬂanks in crack propagation

direction Δu1. Because of local asymmetric deformation, this displacement varies along the crack propagation direction as shown schematically in Fig. 5. This asymmetry in deformation can be found in all microcrystalline materials and especially at loading conditions near the threshold of the stress intensity range. This asymmetry in the volume rotation is clearly visible from electron backscattering diffraction measurements, which deliver crystal orientation maps near the crack ﬂanks. An example is shown in Fig. 6. From this map, it is evident that • The orientation of the crystal changes in the vicinity of the crack ﬂanks, as expected from the consideration earlier. • The amount of the orientation changes is usually different at both sides and changes from grain to grain. Hence, a misﬁt between the two crack ﬂanks remains. Such experimental results are also reﬂected by analytical models.69 Figure 7 illustrates the displacement contour of a crack in the unloaded state after idealized asymmetric deformation. The case can be described by an exact analytical solution, and for simplicity, all dislocations are arranged in a row at 10 μm distance from the crack ﬂanks to mimic the idealized asymmetric case (Fig. 7a). For the calculation of the fracture surface contour, the contact has not been taken into account. Therefore, crack ﬂanks near the crack tip overlap as shown in Fig. 7b. The size of the overlap region is equal to the assumed size of the monotonic plastic zone. This exact analytical description of the displacement ﬁeld supports the ideas presented for the plasticity-induced crack closure under plane strain condition.50,51 The displacement difference between the upper and lower crack ﬂank Δu1 (Fig. 7c), which in the case of a rough fracture surface would lead to a roughness-induced crack closure, increases with increasing distance from the crack tip and then remains nearly constant for distances larger than the plastic zone size. A consequence from these analyses is that besides the roughness of the fracture surface,28 the asymmetry of the plastic deformation in the plastic

Fig. 5 Illustration of the origin of the residual displacement difference Δu1 between the fracture surfaces. (a) From the dislocation point of view, the crystal anisotropy in the wake of the crack causes an asymmetric arrangement of the geometrically necessary dislocations.69 (b) From the continuum mechanics view, an asymmetric plastic zone develops in the crack wake. The variations in the displacement ﬁeld on opposite sides of the crack wake are displayed by red (5a) and white (5b) lines. [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

FATIGUE CRACK CLOSURE

477

zone is larger than the grain size, that is, the monotonic plastic zone contains many grains, the asymmetric deformation resulting from the crystal anisotropy is reduced. A simple estimation of the local misﬁt of fracture surfaces Δu1 is given by Δu1 ¼ α x2 ¼

Fig. 6 Inverse pole ﬁgure maps (crystal orientation map, where the colour code represents the crystal orientation in respect to the macrocrack propagation direction) in the wake of a fatigue crack, 1/2 grown at ΔK = 4.5 MPam at R = 0.1 in pure copper. The crack path is marked by a white line. The change of the colour is a measure for the orientation change, that is, the lattice rotation. The difference in the change of the colour (the rotation) on both sides of the crack is responsible for the misﬁt of the rough fracture surfaces. (For interpretation of the references to color in this ﬁgure legend, the reader is referred to the web version of this article.) [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

wake69 is the essential ingredient that controls roughness-induced crack closure. This is the reason that roughness-induced crack closure is more pronounced in coarser grained materials near the threshold,68,70–72 as long as the monotonic plastic zone size is comparable with the grain size or smaller. If the size of the plastic

b x2 d1

;

(2)

where α is the difference in the rotation angle between the upper and lower plastic wake and x2 the distance over which this ‘rotation’ takes place. Here, b is the length of the Burgers-vector and d1 the distance between the dislocations (Fig. 7a). Hence, a large asymmetry in the plastic deformation (large α) and a large zone where this asymmetry takes place are important to obtain a high contribution of roughness-induced crack closure. This seems to be the reason why in ultraﬁne grained and nano-crystalline metals, despite a high roughness on the nanoscale, no roughness-induced crack closure takes place,73,74 because according to (2), x2 is restricted by the grain size. The discussed mechanisms to explain the roughness-induced crack closure are important for microcrystalline metallic materials in the near threshold regime where the asymmetry in deformation is more pronounced. As mentioned at higher ΔK, the asymmetry of the crack tip deformation is reduced. However, fracture surface roughness, crack branching and delamination can result in a local reduction of the stress

þ Fig. 7 Calculated displacement of the upper and lower crack ﬂank uþ 2 , u2 and u1 and u1 , respectively. The index +, refers to the ‘upper’ and ‘lower’ crack ﬂank. The idealized dislocation arrangement in the crack wake is shown in (a). (b) u2-displacement contour. A contact of the fracture surface is not taken into account, therefore near the crack tip the two crack ﬂanks overlap. (c) u1-displacement contour. After few 69 microns behind the crack tip, the difference between uþ [Colour ﬁgure can be viewed at wileyonlinelibrary.com] 1 and u1 remains constant.

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

478

R. PIPPAN AND A. HOHENWARTER

triaxiality or to a local more plane stress state deformation. This can lead again to an in and out-of-plane ﬂow of material and form an additional plastic wedge. This type of mixed roughness and plasticity-induced crack closure has been discussed elsewhere.75 Oxide-induced crack closure The volume of oxides or other corrosion products is typically larger than the volume of the corresponding base material. Hence, the forming of an oxide layer or corrosion debris on the fracture surface can be interpreted as a wedge which is inserted into the crack. Hence, the reduction of the effective stress intensity range due to the oxide-induced crack closure is straight-forward. The importance of the crack closure because of fracture surface oxidation has been pointed out by a vast number of researchers (for example, Refs. [32–36]) at ambient and at elevated temperatures. The presence of an atmosphere leads to oxidation of freshly formed fracture surfaces, which is often more pronounced in a moist atmosphere.35 The thickness of the oxide layer on a freshly formed surface in most metals and alloys is only a few nanometre at ambient temperatures. Because of the fracture surface contact by plasticity and roughness-induced crack closure, the thickness of the oxide layer can signiﬁcantly increase. The continuous breaking and reforming during the contact and fretting can lead to a build up of oxide layers in the order of 100 nm. This build up of thick oxide layers on the fracture surface is very pronounced at low R-ratios and very low crack growth rates, that is, near the threshold. In steels, these thick oxide layers formed at such loading condition can easily be seen with the naked eye on the fracture surfaces due to their black appearance. The oxide-induced crack closure is important for the explanation of different phenomena near the threshold: • The effect of environment, for example, the observation of the larger ΔKth at low R ratios in moist air.35 • The effect of loading procedure to induce a pre-crack on the measured ΔKth72,76,77 • Unexpected load history effects, for example, load amplitudes below the threshold can reduce the growth rates during the following loading.77 Asperity versus wedge-induced crack closure Herzberg et al.78 performed fatigue crack growth experiments with single artiﬁcial contacts. At relatively large distances from the crack tip (between 10 and 20 mm), shims of different thickness were inserted in the mouth of the opened crack. The reduction in the crack growth rate after introduction of the shims was signiﬁcantly smaller than expected from the measured KmaxKop values.

Riemelmoser et al.54 studied the effect of different asperity geometries on the local stress intensities for linear elastic loaded fatigue cracks. In Fig. 8a, the dotted line shows the contour of the crack at the ﬁrst contact between the asperity and the crack (K = Kcl) and the full line when the remote load is zero. It should be noted that in this ﬁgure, the scale of the displacement in the x2 direction is enlarged by a factor of 100. The width of the assumed asperity is 1/1000 of the distance between the crack tip and the contact (the asperity). From this ﬁgure, it is evident that during further unloading (K < Kcl), a signiﬁcant deformation, that is, reduction of the local stress intensity occurs. In the unloaded case, the local k is not Kcl but only a small portion of Kcl. The contribution to the shielding of the crack tip is only 0.21 (KclKmin). This is in good agreement with the observation of Herzberg78 and the conclusion drawn by Louat.44 In Fig. 8b, the effect of multiple asperities, where the contour of an unloaded crack with four small asperities, is plotted. The four asperities are located at 1000, 2000, 4000 and 8000 times the width of the contact, and the height is chosen in such a way that all asperities close at the same stress intensity factor. Figure 8b illustrates that the crack tip shielding by these four very small contacts is signiﬁcantly larger compared with the single asperity in Fig. 8a. This increase in crack tip shielding with increasing number of contacts is plotted in Fig. 8c. Equidistant, small asperities have a width of 1/1000 of the distance between the crack tip and the ﬁrst contact. It can be seen that 10 very small contacts can cause a crack tip shielding of about 70% of (KclKmin). A similar behaviour is observed when the width of the contacts is increased. Figure 8d shows the contour of the unloaded crack, where the width of the contact is equal to the distance between the beginning of the contact and the crack tip. The height of the contact is equal to the crack tip opening displacement at the closure stress intensity factor. A comparison with the contour of the very small contact in Fig. 8a clearly shows that the elastic relaxation of the crack tip of the unloaded crack is signiﬁcantly reduced by the increase of the width of the contact; the shielding of the unloaded crack tip is in this case about 80% of (KclKmin). In contrast to single asperities, a contact that continuously closes from the crack tip, denoted as wedge-like contact, can completely shield the crack tip. Such wedges-like contacts are depicted in Fig. 9. However, the wedge must have a certain width, otherwise, the stresses at the contacts will be too high, and the wedge will be ‘plastically compressed’. A simple estimation of the minimum size of a wedge causing a complete shielding, that is, no cyclic plastic deformation should

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

FATIGUE CRACK CLOSURE

479

Fig. 8 (a) Illustration of the crack contour at the contact load and at zero load; the width of the asperity is 1/1000 of the distance between the asperity and the crack tip. (b) Crack contour of an unloaded crack with four asperities with a width of 1/1000 of the distance between the ﬁrst asperity and the crack tip. (c) Increase of the local stress intensity with increasing number of equidistant asperities (thickness of the asperities is also 1/1000 of the distance between the ﬁrst asperity and the crack tip. (d) Effect of the increase of the asperity width on the crack contour. The assumed width of the asperity is equal to the distance from the asperity to the crack tip. The large effect of the width on the local k is visible by comparing (a) and (d); see also Refs. [53, 54].

take place, is illustrated in Fig. 9.51,53 At maximum load, an artiﬁcial wedge with different sizes is inserted immediately behind the crack tip. In order to estimate the minimum length of such a wedge, the Dugdale model55 and the McClintock–Rice superposition principle24 are used. In the Dugdale model, the plastic zone is replaced by a narrow strip that extends a distance ω ahead of the crack tip and is loaded by tractions equal to the yield stress σ y over a length xmin. During loading, the tractions cause a negative stress intensity factor equal to the stress intensity factor induced by the applied far-ﬁeld loading. The cyclic plastic zone of a closure free crack is given in the same way as the monotonic plastic zone, with the difference that the loading parameter is replaced by the stress intensity range and the tractions by twice the yield stress. Figure 9e shows the reduction of the cyclic crack tip opening displacement with increasing size of such an artiﬁcial wedge, which also can transfer stresses up to the yield stress of the material. If the deformation during complete unloading should be prevented by a wedge with the minimum width xmin, the tractions induced by the wedge should cause the same stress intensity factor as the far-ﬁeld loading at maximum load. Therefore, the

calculation of xmin is identical with the derivation of the monotonic plastic zone size. Hence, the minimum length of the wedge required to induce a complete shielding is equal to the size of the monotonic plastic zone (xmin = rpl) or 4Δrpl of the closure free crack. A consequence of this simple estimation is that one always needs a certain crack extension to build-up crack closure, not only for the wedge-like contacts of the plasticity-induced or oxideinduced crack closure but also for the roughness-induced crack closure. Real cracks at low stress ratios have both type of contacts, asperity-like and wedge-like contacts. The aforementioned estimations show that only from the single (or few) asperity-induced crack closure a determination of ΔKeff = KmaxKcl overestimates the effect of crack closure and underestimates the resulting crack propagation rate. However, in most cases, the main problem is not whether the crack tip is shielded completely below Kcl or not, but rather the experimental determination of Kcl itself, because it is very difﬁcult to detect the ﬁrst fracture surface contact near the crack tip accurately. The length scales involved in this process are quite small as demonstrated in the next section.

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

480

R. PIPPAN AND A. HOHENWARTER

Fig. 9 Illustration of the minimum length of a wedge ﬁlled into the crack to obtain a certain crack tip shielding. The used Dugdale model is shown in (a) to (d). (a) Crack tip contour of a closure free loaded crack. (b) Conﬁguration of the completely unloaded crack respectively. (c) and (d) present the effect of an inserted wedge on deformation. (e) Decrease of the cyclic crack tip opening displacement with increasing width of the wedge compared with the cyclic crack tip opening displacement without closure.53

The length scales of fatigue crack propagation

ΔCTOD ¼ d n

The length scales involved in fatigue crack propagation are the physical crack length a (notch depth D plus the physical crack length l ), the size of monotonic plastic zone rpl, the size of the cyclic plastic zone Δrpl, the distances between the fracture surface contacts and crack tip, the width of the contacts, the cyclic crack tip opening displacement, the crack growth rate and the characteristic lengths of a microstructure, which can vary from nanometre to metre, depending on loading condition, the component size, sample size and material. Assuming small-scale yielding, which requires that the plastic zone size rpl is much smaller than the crack length and ligament width, the plastic zone size using the Irwin estimation is

ΔK 2 : E2σ y

(5)

These relations apply when no crack closure occurs, where E is the Young’s modulus, σ y is the yield stress and dn is a dimensionless constant that depends on the stress state, very strongly on the hardening exponent n (for a non-hardening material, it is 1 for plane stress and 0.78 for plane strain, and for a high n, it can decrease to about 0.1) and slightly on σ y/E; see Refs.[79, 80]. If crack closure takes place, ΔK has to be replaced by ΔKeff: Δr pl ¼

ΔK 2eff

(6)

π4σ 2y

and K2 r pl ¼ 2 : πσ y

(3)

The cyclic plastic zone size

Δr pl ¼

ΔK 2 π4σ 2y

and the cyclic plastic crack tip opening displacement

(4)

ΔCTOD ¼ d n

ΔK 2eff E2σ y

(7)

The large variation of the length scales is clearly evident from the estimation of the characteristic parameters controlling fatigue crack propagation in Table 1. It has to be noted that the estimation of ΔCTOD near the threshold by Eq. 5 signiﬁcantly overestimates the value; hence, the variation is even larger.81 This indicates that characteristic dimensions vary between nanometre and metre,

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

FATIGUE CRACK CLOSURE

481

Table 1 Illustration of the variation of the size of plastic zone, rpl, for stress ratio R = 0, the size of the cyclic plastic zone Δrpl and cyclic crack tip opening displacement ΔCTOD using the estimations of Eqs 3–5, crack closure for the cyclic values are not taken into account

Near threshold ΔK = 5 MPam1/2

rpl Δrpl ΔCTOD

High Paris regime ΔK = 70 MPam1/2

Low strength steel σ y = 250 MPa

High strength steel σ y = 1800 MPa

Low strength steel σ y = 250 MPa

High strength steel σ y = 1800 MPa

120 μm 30 μm 180 nm

2.4 μm 600 nm 25 nm

26 mm 6.6 mm 36 μm

0.5 mm 0.12 mm 5 μm

which causes the difﬁculties in the experimental and the theoretical analyses of crack closure and fatigue crack propagation phenomena. Experimental measurement of crack closure For the discussion of the experimental evaluation, the vast number of techniques can be divided into three groups: • compliance techniques • crack propagation techniques • non-mechanical contact measurements. Each technique has its advantages and speciﬁc limitations. However, common for nearly all is the problem of measuring the ﬁrst contact very near the crack tip, especially at very small load amplitudes. Figure 10 shows the calculated contour of a crack at minimum load. The simulated crack is grown at constant ΔK over a distance of about 6 μm. The applied discrete dislocation simulation52,81 represents an ideal plane strain loading, and the calculated contour of the crack is the sum of the exact analytical displacement solutions of the simulated dislocation arrangement at the minimum load. During the propagation of the crack, the cyclic crack tip opening displacement ΔCTOD decreases from initially about 50 nm to about 35 nm. This continuous reduction of ΔCTOD and the increase of the contact length to about 1.5 μm cause a decrease of the effective stress intensity range ΔKeff from the initially applied ΔK to about 0.8 ΔK.82 The measurement of crack closure over such a small distance is very difﬁcult and for most experimental techniques impossible to measure; however, for simulation techniques, it also becomes very cumbersome. How fast plasticity-induced crack closure under plain strain conditions is built up even for large ΔK-values is demonstrated in Fig. 10b, where the decrease of the striation spacing directly indicates the decrease of ΔKeff. The compliance technique measures the mechanical response of the contact forces. There are many different techniques to measure the displacement or the local strain: • mechanical strain or displacement gauges, which can be used in a far-ﬁeld or near crack tip arrangement (for example, Refs. [53, 78, 83–86]),

Fig. 10 (a) Illustration of the calculated crack contour by discrete dislocation simulation for a loading case near the threshold with a constant load amplitude.53 The very small closure over a length of about 1.5 μm has signiﬁcantly reduced the cyclic crack tip deformation from about 50 nm of the closure free crack at the beginning to about 35 nm after a crack extension of about 6 μm. (b) Fractograph of a fatigue fracture surface generated in the ﬁrst few 1/2 hundred cycles at ΔK = 70 MPam in a cold worked 316 L austenitic steel. The right side shows the fracture surface of the pre-crack generated at a small ΔK. The reduction of the striation spacing illustrates the fast building up of the plasticity-induced crack closure under plain strain conditions similar as the simulation in (a), which demonstrated the effect at small ΔK. [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

• interferometric displacement measurement,87–89 • in situ optical microscope or in situ scanning electron microscope observation,89–94

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

482

R. PIPPAN AND A. HOHENWARTER

• in situ X-ray tomographic techniques,95–97 • in situ X-ray stress or strain measurements.95,97 Near crack tip techniques are usually more sensitive to measure the fracture surface contacts. However, for some of them, the sensitivity depends strongly on the distance between the sensor and the crack tip and the contact.86 The typical load displacement or load strain curves are depicted in Fig. 11. In the case of a single asperity located at larger distances from the crack tip, a well-pronounced single change of compliance should be observed (Fig. 11a loading case α). But real fatigue cracks close continuously from the crack tip, caused by plasticity-induced crack closure (and maybe by oxide-induced crack closure) and some asperities caused by roughness-induced crack closure or corrosion debris, which results in a continuous change of the compliance (Fig. 11a loading case γ). In addition, the cyclic plastic deformation and friction of the fracture surfaces result in a small hysteresis of the load displacement or the load strain curve (compare with Fig. 11a loading case δ), which makes the determination of Kcl even more difﬁcult. Only a measurement of the strain, the stress or the displacement very near the crack tip permits accurate determination of the fracture surface contact near the crack tip and to determine accurate the effective fatigue crack driving force (Fig. 11b). When the crack closes over larger distances, the evaluation of the Kcl is more straightforward. Hence, in most cases, the problem to determine ΔKeff is not that Kcl overestimates the real ΔKeff due to asperity contacts as shown in the last section, but rather the experimental difﬁculties with the detection of the near crack tip contacts. The second group of techniques, the crack propagation techniques, are based on the assumption that a crack

does not propagate when it is closed, and it can only propagate if ΔK is larger than ΔKeff,th, and Kmax is larger than the Kcl + ΔKeff,th.53,98 Two possible loading procedures to determine Kcl by such method are shown in Fig. 12. In both cases, the crack growth experiments are interrupted at Kmin. In the technique depicted in Fig. 12a, at ﬁrst, a very small ΔK, although larger than ΔKeff,th, is applied and increased in steps until the crack starts to propagate. From the ΔK value where the crack starts to propagate, the Kcl can be calculated with Kcl = KmaxΔKeff,th. Another possibility (Fig. 12b) is to apply a small ΔK, which is somewhat larger than ΔKeff,th and increase the mean load until the crack starts to propagate. Kcl can be determined in the same way as in the ﬁrst technique. A result of such somewhat modiﬁed experiment is shown in Fig. 13a and b, which was used to determine the crack closure load during constant amplitude loading in an austenitic steel. The difference between the loading procedure shown in Fig. 12b and the used one in Fig. 13a is that after each small load step, few constant load amplitudes of the base loading were applied. The resulting fatigue fracture surface is presented in Fig. 13b. Because of the well-formed striations generated during the base loading, the load step where the ﬁrst crack propagation occurred can be clearly detected (load block C), and Kcl can be determined very accurately from the relation Kcl = KmaxΔKeff th. For comparison, the very near crack tip opening displacement measured with a special compliance technique obtained from direct measurement of the crack tip deformation was used at the same ΔK and R-ratio (Fig. 14). The two independent measurements of the closure load are in good agreement. At this relatively large ΔK, oxide-induced and roughness-induced

Fig. 11 Schematic illustration of load versus crack opening displacement curves.53 (a) Effect of different contacts, α: single contact at larger distances from the crack tip, β: two contacts at different distances behind the crack tip, γ: a continuous closing crack and δ a continuous closing crack where cyclic plastic deformation and friction between the fracture surfaces takes place. (b) Inﬂuence of distance between contact and the position where the displacement is measured. The position of the measurement and the corresponding compliance record are depicted in the schematic. [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

FATIGUE CRACK CLOSURE

483

Fig. 12 Schematic representation of the loading procedures to measure the crack opening load, Kop, after Ref. [89]. [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

crack closures are not relevant, and the plane strain conditions were fulﬁlled, therefore these experiments clearly support the existence of the plasticity-induced crack closure under plane strain during constant amplitude loading. Kcl is about 0.25 Kmax in the plane strain case, which is in good agreement with the results of the ﬁnite element simulations (for example, Ref. [100]). It should be noted that this is signiﬁcantly smaller than for the plane stress case where Kcl at R = 0 is about 0.5 Kmax. The third group of techniques try to measure the occurrence of a contact by optical,86–89 acoustic101 or electrical methods.102 In transparent materials, optical technics can be used to determine both the change of crack tip opening displacement during the load cycle by a Newton interference method and determine the contact area and location.88,89 The acoustic methods use the change of transmission or reﬂection of acoustic waves

from closing crack ﬂanks.101 The advantage of these methods is that they permit a through thickness evaluation of the closure process. Furthermore, the acoustic emission when the crack faces come into contact has been used to determine the closure load. The electrical resistivity of the oxide layer on the fracture surface of most metals and alloys is very high; therefore, the change of the potential drop during the fracture surface contact is very small. Only for fatigue crack propagation in high or ultra-high vacuum the closure of the fracture surface contacts signiﬁcantly effects the potential drop.102 But few friction contacts of the fracture surface causes potential drop changes during the whole loading range, which makes the determination of the mechanically effective contacts difﬁcult. Similar problems arise in the use of the acoustic emission method.

Fig. 13 (a) Modiﬁed loading procedure to measure the crack opening load with crack propagation technique in materials with a well-deﬁned striation appearance in fatigue. (b) The resulting fatigue fracture surface of such a test53, the ﬁrst crack extension at the small load is clearly visible at the load block C. [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

484

R. PIPPAN AND A. HOHENWARTER

Fig. 14 Crack tip opening displacement, measured in the midsection of the thick specimen, 2 μm behind the crack tip determined in a constant ΔK test with R = 0.05 by means of a special stereophotogrammetric technique.99 The measured crack tip opening indicates the closure of the crack at 22% of the maximum load, even at this large ΔK-value where only plasticity-induced crack closure is active. The experiments were performed with the same material as in Fig. 13, and the determined closure values are in good agreement. [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

Prediction of crack closure For materials where the fatigue crack propagation is solely governed by the cyclic plastic deformation, which is typical for ductile materials and for loading signiﬁcantly below the fracture toughness, the knowledge of the effective stress intensity range or the effective ΔJ should be sufﬁcient for the prediction of the fatigue crack growth rate. Therefore, the description of the • mean stress or load ratio effects, • the effects of load history, that is, the effect of overloads, underloads and variable amplitude loading, • and the effect of physically short cracks is fundamentally related to the changes of the crack closure. The prediction of the crack closure load along with the knowledge of da/dN versus ΔKeff are the essential ingredients for an accurate lifetime calculation. The different approaches to predict crack closure can be divided into • strip yield models, • elastic plastic ﬁnite element analyses and • analytical or half-analytical models, which are partly physically or empirically related. The prediction of crack closure and the lifetime prediction in general under variable loading is a very broad ﬁeld, and the goal of this section is not to review all of the studies. Here, only the possibilities and limitations of the different groups are shortly summarized, and some important open questions will be pointed out. The strip yield models are based on the Dugdale model. The ﬁrst models of this type were introduced by

Führing and Seeger,57 Newman58,103 and de Koning.59 The numerical simulation uses thin strip elements along the crack line. These strips in the plastic zone ahead of the crack are intact and carry both tension and compressive stresses. The elements in the wake are broken and can only carry compressive stresses during the loading phase when they are in contact. Outside the strip, the material is perfectly elastic, like in the Dugdale model. During unloading, the contact stresses are computed. The displacement of the strip (height of the bar elements which form the plastic wedge) is adapted if the stress is larger than the yield stress. The main difference between the models is how the constraint is taken into account in order to mimic plane stress or the plane strain conditions; for details, see Refs. [62, 66, 100]. The strip yield model is a good physical approximation for the description of the plasticity-induced crack closure under plane stress conditions. However, for fatigue crack propagation under plane strain conditions, it does not reﬂect the real physical phenomena (see again Fig. 2). By varying the constraint parameters in the model, a somewhat thinner wedge can be obtained to mimic a more local wedge, which is typical of the plane strain case (Fig. 3a). Numerous ﬁnite element or boundary element analyses have been performed to simulate fatigue crack growth (for example, Refs. [103–115]). Most of these studies were conducted to obtain a basic understanding of the crack closure mechanisms and how the crack tip stress and strain ﬁelds are inﬂuenced by the plastic deformation in the plastic zone and the wake of the crack tip. The majority of these studies were performed either under plane stress or plane strain conditions. Only a relatively small number of three-dimensional ﬁnite element analyses (for example, Refs. [104–106] of fatigue crack propagation have been performed. The vast majority of these studies focused on plasticity-induced crack closure, only a few attempts have been made to simulate roughness-induced and oxide-induced crack closures.108,109 One of the most crucial points is the element type and mesh size,110–117 which is especially significant for the plane strain case, where the plastic ‘wedge’ is very short. The mesh size is critical and may be one of the main reasons for the discrepancies observed under plane strain conditions. Because of the extended wedge under plane stress, this point is not as crucial. Most of the studies are performed for a speciﬁc cyclic and monotonic material behaviour, and only very few studies consider a monotonic and cyclic hardening or softening118–120 as well as ratchetting.121 Only the effect of the ratio of the loading stress to yield stress has been investigated in detail (for example, Refs. [100, 105, 120]). The general trend of these analyses shows that with an increasing ratio of applied stress to yield stress, the ratio of the closure stress to applied stress decreases. Only in the well-

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

FATIGUE CRACK CLOSURE

deﬁned small-scale yielding regime under constant amplitude loading the closure stress intensity factor depends only on the stress ratio. This clearly demonstrates that crack closure is a consequence of the encapsulated plastic deformation in an elastic surrounding. The ﬁnite element method is the best tool to study all material parameters and loading parameters as well as the 3D effects that inﬂuence the plasticity-induced crack closure. However, more research is needed to draw a clear quantitative picture of the load, load interaction effects and the inﬂuence of the plastic behaviour of the material on plasticity-induced crack closure, which is the only effect that should be described without assumptions. With such basic knowledge, other, not as cumbersome, tools such as the strip yield method or other more analytical tools could be calibrated. In the third group, we have summarized a large number of methods that usually do not examine the details of the closing and opening phenomena of the crack or the details of this effect on the cyclic plastic deformation. Some of them are physically based, others are a purely empirical description by ﬁtting of experimental observations, like the NASGRO equation (for example, Refs. [122–124]). By combining empirical relations such as the Wheeler model124 with the closure behaviour, or using dislocation shielding concepts, one could attempt to predict the load history effects (for example, Ref. [65]). As already mentioned previously, from a physical point of view, only the plasticity-induced crack closure can be predicted without questionable assumptions. For example, a physical prediction of the roughness-induced crack closure would require a detailed description of the fatigue crack propagation by crystal plasticity over a large growing distance compared with the characteristic microstructural dimensions and an assumption of the roughness details of fracture surface. A description of the oxide-induced crack closure would require information of the growth of the oxide layer or asperities as a function the contact type, the friction, the contact load, the environment and the evolution of the oxide growth process during the cyclic loading. Most of these details required for the prediction of the roughness-induced crack closure and the oxide-induced crack closure are unknown. Therefore, some of the empirical models are useful because they incorporate all three closure mechanisms. But even for the simple constant amplitude loading (see the schematic in Fig. 15), a simple description for the oxide-induced and roughness-induced crack closures as a function of ΔK, the stress ratio R and the environment does not exist. Even for the most simple case of load interaction of a single overload in the mid Paris regime, where roughness-induced and oxide-induced crack closures are

485

Fig. 15 Schematic illustration of the effect of oxide-induced, roughness-induced and plasticity-induced crack closures on the fatigue crack propagation behaviour (da/dN versus ΔK) in ductile materials, where ΔKeff controls the fatigue crack growth rate. [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

insigniﬁcant, the experimentally observed retardation effects cannot be fully predicted by the present models. Figure 16 shows the experimental results of overload experiments on samples with very different thicknesses.99 The strong thickness effect is evident. In the 25-mmthick sample, the overload plastic zone is dominated by the plane strain state. In the 9-mm-thick sample, the overload plastic zone is mainly dominated by the plane stress state, whereas the cyclic plastic zone during the unloading from the overload and the monotonic plastic zone during the base loading are dominated by plane strain. In the thinnest sample (3 mm), only the cyclic plastic zone during base loading is dominated by the plane strain state, the others are dominated by the plane

Fig. 16 Effect of specimen thickness (i.e. stress state in the plastic zones) on the retardation effect after a single overload.99 The base 1/2 load amplitude was 70 MPa·m , the effect of stress state, is even visible in the steady state fatigue crack propagation rate. The crack propagation rate was determined from the striation spacing. [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

486

R. PIPPAN AND A. HOHENWARTER

stress state. These experimental results and estimations of the deformation conditions, which have to be taken into account for an accurate prediction of the propagation behaviour, reﬂect the complexity of this simple loading case. Only a careful 3D ﬁnite element simulation of the different loading cases could deliver a description of the observed phenomena. Besides the loading effect, the inﬂuence of how the plastic properties of the material as cyclic and monotonic hardening or softening affect this phenomena is not analysed in detail. Despite the importance of the prediction of crack closure, it is surprising that such basic open questions are not satisfactorily solved.120,125–128 Crack closure versus compressive residual stress It is well known that residual stresses signiﬁcantly affect the fatigue crack propagation behaviour.1,30,129–131 Macroscopic residual stresses can be considered as an additional applied static loading, and they change locally the stress ratio. In special cases, the effect of the residual stresses on the fatigue crack propagation rate can be used to estimate these local variations of the residual stresses.131 Because of plastic deformation in front of the crack in an unloaded sample or component, always a characteristic residual stress ﬁeld remains, depending on the applied load history. During changes of the load amplitude, the residual stress ﬁeld changes. There are several authors which try to describe the load interaction effects solely by changes of the residual stresses in front of the crack. In principle, such approaches could be used to take into account all effects – stress ratio, load interaction or physical short crack effects. However, a detailed description of the residual stresses including the contact stresses at the minimum load in each load cycle should be incorporated. Such approach is more or less equivalent with a detailed description of the cyclic plastic deformation in front of the crack tip in each cycle, which is very difﬁcult. In order to avoid the cumbersome calculations, simple estimations are introduced, which can reﬂect some observations during variable amplitude loading.132–134 However, several details cannot be described with such simpliﬁcations of the effect of the residual stresses in front of the crack. For single overload, the arising problems will be shortly discussed. A sufﬁcient large overload induces a ‘residual blunting’ that opens the crack (for example, Ref. [99]. Because of the additional plastic deformation induced by the overload, a larger zone with compressive residual stresses develops. These larger compressive residual stresses are used to explain the retardation effect.132–134 The largest residual stresses in front of the crack are present immediately after the overload, hence the largest reduction of the crack propagation rate should be observed immediately after the overload.

However, in the ﬁrst few cycles after the overload, cracks propagate faster than before the overload (Fig. 16), and then the crack growth rate decreases below the growth rate of the base amplitude loading; this phenomenon is usually called the delayed retardation. Because of the more extensive blunting at the overload, the fracture surface contact is reduced or disappears completely, which causes the initial increase of the crack propagation rate. On the new fatigue fracture surface generated in the loading cycles after the overload, the fracture surfaces come again into contact, and compressive stresses are transferred; this leads to a continuous decrease of the growth rate.99 Because of larger plastic deformation at the overload, the contact stresses and the region where this contact stresses act are larger than during constant amplitude loading. In other words, the closure load is larger than during the base loading, or the effective stress intensity range is smaller than during base amplitude loading. If not only the residual stresses at the minimum load in front of the crack but also the fracture surface contacts were taken into account, the residual stress concept would allow to describe the delayed retardation and would be more or less equivalent to the closure concept.

Physically short crack effect Short cracks grow often signiﬁcantly faster than long cracks and can propagate below the long crack threshold stress intensity range. This was ﬁrst presented by Pearson.40 A vast number of papers and several conferences are devoted to this important problem. In order to understand the different phenomena, it is very helpful to divide the different short cracks41,135 into classes. • For microstructurally short cracks, the crack size is comparable or smaller than the characteristic microstructural dimension, such as the grain size or the spacing of different phases in composites. • For mechanically short cracks, the plastic zone size is in the order of the crack length or larger, so that smallscale yielding is not fulﬁlled, which is often the case during low and high cycle fatigue testing of smooth specimens. How crack closure changes for this class of cracks will be discussed in the next chapter. • Fatigue cracks or ﬂaws in components where smallscale yielding is applicable but crack tip shielding mechanisms not fully developed are denoted as physically short cracks or extrinsically short cracks. • In aggressive environments, cracks below a certain crack size behave differently and are termed chemically short cracks. This is caused not only by a change of the chemical transport in the crack but also by a change of asperity-induced crack closure.

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

FATIGUE CRACK CLOSURE

Cracks emanating from small ﬂaws or sharp notches usually are initially open over the full load range. With crack extension, the newly generated fatigue fracture surface can come into contact, and the closure stress intensity factor increases. This corresponds to the physically short crack case. Figure 17 shows the fatigue crack propagation behaviour on very sharp deep notches, in ARMCO iron (technically pure Fe). The experiments are performed at constant ΔK at different stress ratios. At stress ratios between 0.5 and 1,136 the crack growth rate is independent of the crack length measured from the notch root. For smaller stress ratios, the growth rate decreases till it either becomes constant or drops towards zero. For very short crack extension, the crack growth rate is independent of stress ratio and independent whether the experiment is performed in remote compression loading (R = 2;∞), tension–compression (R = 1) or in tension loading (R = 0.1; 0.5), that is, the effective driving force is always ΔK or Kcl = Kmin. These experimental results clearly show that only the cycle deformation determines the crack propagation behaviour, or in other words, the contribution of the monotonic deformation can be ignored in this ductile materials at these relatively low ΔK values. A similar behaviour can be also seen on the fractograph in Fig. 10b, where the initial decrease of the growth rate due to the building up of crack closure at the beginning loading block with a large load amplitude is clearly visible. The reduced effect of crack closure in physically short cracks is responsible for the abnormal fast crack growth

Fig. 17 Illustration of the fatigue crack propagation behaviour in deep sharp notched specimens (crack-like notches) as a function of crack length measured from the notch root at constant ΔK = 16 and 1/2 6 MPa·m and different stress ratios. R = ∞ means pure cyclic compression. The experiments were performed with pure iron (ARMCO iron). For further details, see Ref. [136]. [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

487

and the crack propagation below the long crack threshold. Therefore, the crack growth of physically short cracks could be either described by the increase of crack closure or can be interpreted as an R-curve behaviour of fatigue cracks. In fracture mechanics, the increase of the fracture resistance is denoted as an R-curve behaviour. Such R-curves are depicted in Fig. 18.137 It shows the necessary ΔK to obtain a certain crack propagation rate. Such R-curves for different growth rates are unusual, because they are difﬁcult to measure. An exception is the R-curve for the threshold of stress intensity range, which represents the R-curve for da/dN = 0.42,72,75,137–139 A relatively simple technique to measure such Rcurves for ΔKth is the stepwise increasing load amplitude test on deep notched specimens.139 The requirement for such measurement is to produce a pre-crack, which is open during the full load amplitude and contains no or at least very small residual stresses in front of the crack. A load procedure to measure such R-curve for ΔKth is shown in Fig. 19. In this case, the pre-crack is generated in pure compression. The load should be as small as possible (hence a sharp notch is required), and the number of cycles should be relatively large to reduce residual stresses to a minimum. The opening stress intensity is in such case about the maximum stress intensity factor of the pre-cracking (which is zero or a small negative value) minus the effective threshold of stress intensity range. If possible, an annealing to reduce further the residual stress is an option. In the stepwise increasing load amplitude test, to measure the R-curve for the threshold, one starts with a very small load amplitude. If ΔK is smaller than ΔKeff,th, no

Fig. 18 R-curve for fatigue crack propagation of ARMCO iron with a grain size of about 70 μm at a stress ratio of 0.1. The data are obtained from constant ΔK tests on deep sharp notched specimens performed at different ΔK-values.137 [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

488

R. PIPPAN AND A. HOHENWARTER

Fig. 19 Illustration of stepwise increasing load amplitude test to determine the R-curve of the threshold of stress intensity range, the long crack threshold and the long crack da/dN versus ΔK behaviour. The loading procedure, the resulting crack extension as a function of number of cycles, the resulting R-curve for ΔKth and da/dN versus ΔK curve are schematically illustrated.139 [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

crack propagation will be observed. If ΔK is larger than ΔKeff,th but smaller than the long crack threshold ΔKth, the crack will start to propagate till the effect of the closure crack reaches a value that ΔKeff ≤ ΔKeff,th. If the load amplitude corresponds to a ΔK larger than ΔKth, the crack will not stop to propagate, and the standard da/dN versus ΔK behaviour can be determined from the crack length versus the number of cycles. ΔKeff,th is between the ΔK values of the load blocks where no crack propagation and the ﬁrst crack propagation is observed which might be difﬁcult to measure, especially in high strength materials, where the R-curve for ΔKth is often very steep. The long crack threshold ΔKth lies between the ΔK values of the load blocks where the crack stops for the last time and the load block where the crack does not stop anymore. From the stopping crack extension and corresponding ΔK, the R-curve for ΔKth can be determined. The increase of ΔKth in such R-curve can be interpreted as the increase of crack closure stress intensity as a function of the crack length at the threshold of stress intensity range (for details, see Ref. [139]). The short crack behaviour is especially pronounced at low and negative R-ratios, because there, the decrease of ΔKeff with increasing crack length is very pronounced. Furthermore, it should be noted that for negative R-ratios, the Kcl (or the closure value) may also depend on the applied minimum stress and not solely on the R-ratio as presented in Fig. 17. Especially pronounced is this effect when the negative applied stresses become into the order of the yield stress,140 because due to the high contact stresses, the contacts may deform plastically, and the closure value decreases, that is, ΔKeff increases.

From small-scale yielding to large-scale yielding For long fatigue cracks under small-scale yielding conditions, the closure load is always a tensile load. Only immediately after an overload or in the case of large compressive contribution with compressive stresses near the yield stress the opening load or closure load is near zero load.141 What happens when the small-scale yielding condition is not fulﬁlled? This question was treated at ﬁrst by Dowling and Iyyer.142 Figure 20 shows this extreme behaviour of the short crack under low cycle fatigue loading. The experiment at constant strain amplitude was performed in a scanning electron microscope91 (SEM). The obtained stress–strain behaviour and the SEM images of the near crack tip regime at the different loads are depicted in Fig. 20. Because of the large strain amplitude, a typical hysteresis of the stress–strain curve is observed. Figure 14 showed also the crack tip opening displacement measured directly at the crack tip of the same austenitic steel (however in a cold worked state) of a long crack under small-scale yielding conditions with comparable cyclic crack tip opening displacement and comparable da/dN; for experimental details, see Ref. [9]. The essential differences between small-scale yielding and low cycle fatigue are as follows: • Under small-scale yielding and constant amplitude loading, the crack closure and crack tip opening loads are about equal, but under low cycle fatigue (LCF) loading, the crack closure and the crack opening stresses are very different. The crack closes near the minimum stress (Position 4) and opens near the transition from compression to tension (between Positions 6 and 7).

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

FATIGUE CRACK CLOSURE

489

Fig. 20 Illustration of the crack closure under low cycle fatigue loading (full-scale yielding conditions). Scanning electron microscope images are taken at different positions of the stress–strain hysteresis curve.91 In this graph, the stresses and strains refer to the uncracked cross-section of the specimen. [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

• For loading with constant strain amplitude, the strain where the crack closes and opens is equal. Hence, for LCF, it makes more sense to deﬁne an effective strain amplitude and not an effective load or stress amplitude. The effective strain amplitude during constant strain amplitude loading is about Δεeff ¼ Δε εy where εy is the elastic component of the strain amplitude Δεel/2. In principle, under small-scale yielding, a deﬁnition of an effective strain amplitude is also useful. Because of the linear relation between stress and strain, it is not important how one evaluates the effective crack driving force by Δσ eff or Δεeff. The consequence of this change of the closure behaviour from the LCF to the small-scale yielding case is schematically depicted in Fig. 21. At large plastic strain amplitudes, considering a strain-controlled experiment, in metallic materials, usually a stress ratio of 1 develops, independent of the starting condition, hence the schematic Fig. 21 is drawn for a stress ratio of 1. It is evident from this ﬁgure that the effect of crack closure is small at a very large strain amplitude and increases with decreasing strain amplitude. In other words, the ratio of the effective driving force to the macroscopic applied crack driving force decreases signiﬁcantly with decreasing plastic strain

amplitude (Fig. 22). This is especially pronounced when the plastic strain amplitude becomes very small. The term crack closure has been originally introduced to incorporate that growing fatigue cracks are not open during the complete tension part of the load amplitude. During LCF loading, the term crack closure is used here somewhat more general, if a crack is closed over a certain part of the strain amplitude. But we have already seen that physically short cracks can be open also during the compression phase of the load amplitude; however, the closure load in this case increases till it reaches the long crack closure value, which is in the tension regime. That is different in the LCF regime, where the effective strain amplitude remains relatively constant independent of the crack extension. The crack closure during LCF loading is simply a consequence of the elastic load bearing capacity of the crack wake. Cyclic creep may shift the opening load into the compression regime. The origin of the crack closure in the LCF regime is therefore different to the crack closure under small-scale yielding condition. Because of the high stresses on the crack ﬂanks, which can lead to a plastic deformation of the crack wake, the roughness-induced and oxide-induced crack closures are of minor importance in this case. A change of the loading amplitude from the LCF to the high cycle fatigue regime and the small-scale yielding regime will change the closure mechanisms from the simple

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

490

R. PIPPAN AND A. HOHENWARTER

Fig. 21 Illustration of the effect of crack closure on the effective crack driving force in the different loading regimes of fatigue crack propagation, from full-scale yielding to small-scale yielding.91 [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

Fig. 22 Effect of crack closure (compressive load-induced closure) on the effective crack driving force in the low and high fatigue regimes.91 [Colour ﬁgure can be viewed at wileyonlinelibrary.com]

compression load-induced crack closure (elastic load bearing of the crack wake) to the plasticity-induced, roughness-induced and oxide-induced crack closures.

CONCLUSIONS

In ductile materials, crack closure is essential to explain the effects of stress ratio, short cracks and load history on fatigue crack propagation. The origin of the plasticity-induced, roughness-induced and oxide-induced crack closures and their consequences for the experimental veriﬁcation and the prediction are reviewed.

• The plasticity-induced crack closure under plane stress and under plane strain conditions require different explanations. For constant amplitude loading, the plasticity-induced crack closure under plane stress conditions can be interpreted as a wedge ﬁlled into the crack, induced by the out-of-plane ﬂow in the plastic zone. In the plane strain case, only a local wedge near the crack tip develops as a consequence of the plastic shear deformation in the plastic wake of the crack. The size of this wedge is in the order of the size of the plastic zone. • Roughness-induced crack closure is a consequence of the asymmetric in-plane and out-of-plane displacements of the crack ﬂanks induced by asymmetric deformation of the plastic wake. • Asperity-induced crack closure does not completely shield the crack tip after the ﬁrst contact because of elastic relaxation of the crack contour between the crack tip and the asperity during the unloading phase. For a large number of asperity contacts, this reduction of crack tip shielding is small, which means that a large number of asperities behaves like a wedge and is well approximated by ΔKeff = KmaxKcl. • Crack tip shielding by crack closure requires a certain width of the fracture surface contact. However, this length can be quite small. A wedge-like contact behind the crack tip of one-fourth of the cyclic plastic zone can induce signiﬁcant reduction of ΔKeff, and a signiﬁcant crack tip shielding. • This relatively small necessary contact width causes the problems in the experimental veriﬁcation of crack closure by far-ﬁeld closure measurement techniques, and also, simulations require a very detailed analysis of the near crack tip deformation.

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

FATIGUE CRACK CLOSURE

• Plasticity-induced crack closure is in principle predictable; however, there are many open questions in the exact prediction, especially the 3D effects, transition from the plane strain to the plane stress case, of the effect of cyclic and monotonic softening or hardening on the closure behaviour of the crack. • Prediction of roughness-induced and oxide-induced crack closures requires extensive additional experimental and theoretical studies. • Crack closure is not only important under small-scale yielding conditions; it plays a crucial role under large-scale yielding as well. In the transition regime, the crack closure load decreases and can decrease into the compression regime of the load amplitude for high and low cyclic fatigue loadings. Acknowledgements Funding of this work has been provided by the European Research Council under ERC Grant Agreement No. 340185 USMS and by the Austrian Science Fund (FWF) in the framework of research project P26729N19.

REFERENCES 1 Ritchie, R. O. (1988) Mechanisms of fatigue crack propagation in metals, ceramics and composites: role of crack tip shielding. Materials Science and Engineering A, 103, 15–28. 2 Laird, C. (ASTM International, 1967). The inﬂuence of metallurgical structure on the mechanisms of fatigue crack propagation. in STP 415 Fatigue crack propagation 131 3 Pelloux, R. M. N. (1970) Crack extension by alternating shear. Engineering Fracture Mechanics, 1, 697–704. 4 Pelloux, R. M. N. (1969) Mechanisms of formation of ductile fatigue striations. ASM Trans Quart, 62, 281–285. 5 Neumann, P. (1974) The geometry of slip processes at a propagating fatigue crack—II. Acta Metallurgica, 22, 1167–1178. 6 Vehoff, H. and Neumann, P. (1980) Crack propagation and cleavage initiation in Fe-2.6%-Si single crystals under controlled plastic crack tip opening rate in various gaseous environments. Acta Metallurgica, 28, 265–272. 7 Tomkins, B. and Biggs, W. D. (1969) Low endurance fatigue in metals and polymers – part 3: the mechanisms of failure. Journal of Materials Science, 4, 544–553. 8 Furukawa, K., Murakami, Y. and Nishida, S. (1998) A method for determining stress ratio of fatigue loading from the width and height of striation. International Journal of Fatigue, 20, 509–516. 9 Bichler, C. H. and Pippan, R. (1999) Direct observation of the formation of striations. Engineering Against Fatigue (Edited by J. H. Begon, M. W. Brown, R. A. Smith, T. C. Lindley and B. Tomkins), pp. 211–218. 10 Siegmund, T., Kolednik, O. and Pippan, R. (1990) Direct measurement of the cyclic crack-tip deformation. Zeitschrift fur Met., 81, 677–683.

491

11 Suresh, S. (1991) Fatigue of Materials, Cambridge University Press: Cambridge. 12 Lawn, B. (1993) Fracture of Brittle Solids, Cambridge University Press: Cambridge. 13 Gilbert, C. J. and Ritchie, R. O. (1998) On the quantiﬁcation of bridging tractions during subcritical crack growth under monotonic and cyclic fatigue loading in a grain-bridging silicon carbide ceramic. Acta Materialia, 46, 609–616. 14 Gilbert, C. J. and Ritchie, R. O. (1997) Mechanisms of cyclic fatigue crack propagation in a ﬁne grained alumina ceramic: the role of crack closure. Fatigue and Fracture of Engineering Materials and Structures, 20, 1453–1466. 15 Gilbert, C. J., Cao, J. J., Jonghe, L. C. and Ritchie, R. O. (1997) Crack growth resistance curve behavior in silicon carbide: small versus long cracks. Journal of the American Ceramic Society, 80, 2253–2261. 16 Pippan, R., Hageneder, P., Knabl, W., Clemens, H., Hebesberger, T. and Tabernig, B. (2001) Fatigue threshold and crack propagation in γ-TiAl sheets. Intermetallics, 9, 89–96. 17 Rao, K. T. V., Odette, G. R. and Ritchie, R. O. (1994) Ductilereinforcement toughening in γ-TiAl intermetallic-matrix composites: effects on fracture toughness and fatigue-crack propagation resistance. Acta Metallurgica et Materialia, 42, 893–911. 18 Pippan, R., Höck, M., Tesch, A., Motz, C., Beschliesser, M. and Kestler, H. (2003) Fracture processes, fracture resistance and fatigue crack propagation in gamma TiAl. In: Gamma Titanium Aluminides 2003 (Edited by Y. W. Kim, H. Clemens and A. H. Rosenberger), pp. 521–529. 19 Tschegg, E. K., Ritchie, R. O. and McClintock, F. A. (1983) On the inﬂuence of rubbing fracture surfaces on fatigue crack propagation in mode III. International Journal of Fatigue, 5, 29–35. 20 Ewing, J. A. and Humfrey, J. C. W. (1903) The fracture of metals under repeated alternations of stress. Philos. Trans. R. Soc. London. Ser. A, Contain. Pap. a Math. or Phys. Character, 200, 241–250. 21 Schijve, J. (2003) Fatigue of structures and materials in the 20th century and the state of the art. International Journal of Fatigue, 25, 679–702. 22 Zapffe, C. A. and Worden, C. O. (1951) Fractographic registrations of fatigue. Trans. Am. Soc. Met., 43, 958–969. 23 Sih, G. C., Paris, P. C. and Irwin, G. R. (1965) On cracks in rectilinearly anisotropic bodies. International Journal of Fracture Mechanics, 1, 189–203. 24 Rice, J. (ASTM International, 1967). Mechanics of crack tip deformation and extension by fatigue. in STP 415 Fatigue crack propagation 247–309 25 Elber, W. (ASTM International, 1971). The signiﬁcance of fatigue crack closure. in STP 486 Damage tolerance in aircraft structures 230–242 26 Elber, W. (1970) Fatigue crack closure under cyclic tension. Engineering Fracture Mechanics, 2, 37–45. 27 Minakawa, K. and McEvily, A. J. (1981) On crack closure in the near-threshold region. Scripta Metallurgica, 15, 633–636. 28 Suresh, S. and Ritchie, R. O. (1982) A geometric model for fracture surface roughness-induced crack closure during fatigue crack-growth. J. Met., 34, 71. 29 Morris, W. L., James, M. R. and Buck, O. (1983) A simple model of stress intensity range threshold and crack closure stress. Engineering Fracture Mechanics, 18, 871–877. 30 Suresh, S. (1985) Fatigue crack deﬂection and fracture surface contact: micromechanical models. Metallurgical Transactions A, 16, 249–260.

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

492

R. PIPPAN AND A. HOHENWARTER

31 Suresh, S. and Ritchie, R. O. (1982) A geometric model for fatigue crack closure induced by fracture surface roughness. Metallurgical Transactions A, 13, 1627–1631. 32 Paris, P. C., Bucci, R. J., Wessel, E. T., Clark, W. G. and Mager, T. R. (ASTM International, 1972). Extensive study of low fatigue crack growth rates in A533 and A508 steels. in STP 513 Stress Analysis and Growth of Cracks 33 Ryder, D. and Lynch, S. P. (1977). The effect of environment and frequency on crack nucleation. Stage I and Stage II crack growth in two aluminum zinc magnesium alloys. in I Mech E Conf. Publ. 21–26 34 Skelton, R. P. and Haigh, J. R. (1978) Fatigue crack growth rates and thresholds in steels under oxidising conditions. Materials Science and Engineering, 36, 17–25. 35 Suresh, S., Zamiski, G. F. and Ritchie, R. O. (1981) Oxideinduced crack closure: an explanation for near-threshold corrosion fatigue crack growth behavior. Metallurgical Transactions A, 12, 1435–1443. 36 Suresh, S., White, C. and Ritchie, R. O. (1980) Oxide-induced crack closure. J. Met., 32, 76–76. 37 McEvily, A. J. (ASTM International, 1988). On crack closure in fatigue crack growth. in STP 982 Mechanics of Fatigue Crack Closure 35–43 38 McKelvey, A. L. and Ritchie, R. O. (2001) Fatigue-crack growth behavior in the superelastic and shape-memory alloy nitinol. Metallurgical and Materials Transactions A: Physical Metallurgy and Materials Science, 32, 731–743. 39 Ritchie, R. O. (1999) Mechanisms of fatigue-crack propagation in ductile and brittle solids. International Journal of Fracture, 100, 55–83. 40 Pearson, S. (1975) Initiation of fatigue cracks in commercial aluminium alloys and the subsequent propagation of very short cracks. Engineering Fracture Mechanics, 7, 235–247. 41 Ritchie, R. O. and Suresh, S. (1983) The fracture mechanics similitude concept: questions concerning its application to the behavior of short fatigue cracks. Materials Science and Engineering, 57, L27–L30. 42 Tanaka, K., Nakai, Y. and Yamashita, M. (1981) Fatigue growth threshold of small cracks. International Journal of Fracture, 17, 519–533. 43 Ritchie, R. O. and Lankford, J. (1986) Small fatigue cracks: a statement of the problem and potential solutions. Materials Science and Engineering, 84, 11–16. 44 Louat, N., Sadananda, K., Duesbery, M. and Vasudevan, A. K. (1993) A theoretical evaluation of crack closure. Metallurgical Transactions A, 24, 2225–2232. 45 Vasudeven, A. K., Sadananda, K. and Louat, N. (1994) A review of crack closure, fatigue crack threshold and related phenomena. Materials Science and Engineering A, 188, 1–22. 46 Riemelmoser, F. O. and Pippan, R. (1998) Discussion of error in the analysis of the wake dislocation problem. Author’s reply. Metallurgical and Materials Transactions A, Physical Metallurgy and Materials Science, 29, 1357–1360. 47 Sadananda, K. and Vasudevan, A. K. (1998) ‘Discussion of error in the analysis of the wake dislocation problem’-Reply. Metallurgical and Materials Transactions A, Physical Metallurgy and Materials Science, 29, 1359–1360. 48 Riemelmoser, F. O. and Pippan, R. (1999) Discussion of ‘reconsideration of error in the analysis of the wake dislocation problem’. Metallurgical and Materials Transactions A: Physical Metallurgy and Materials Science, 30, 1452–1457. 49 Sadananda, K. and Vasudevan, A. K. (1999) Authors’ response. Metallurgical and Materials Transactions A: Physical Metallurgy and Materials Science, 30, 1457–1459.

50 Pippan, R. and Riemelmoser, F. O. (1998) Visualization of the plasticity-induced crack closure under plane strain conditions. Engineering Fracture Mechanics, 60, 315–322. 51 Riemelmoser, F. O. and Pippan, R. (1998) Mechanical reasons for plasticity-induced crack closure under plane strain conditions. Fatigue and Fracture of Engineering Materials and Structures, 21, 1425–1433. 52 Pippan, R., Riemelmoser, F. O., Weinhandl, H. and Kreuzer, H. (2002) Plasticity-induced crack closure under plane-strain conditions in the near-threshold regime. Philosophical Magazine A, 82, 3299–3309. 53 Pippan, R., Riemelmoser, F. O. and Bichler, C. (ASTM International, 1999). Measurability of crack closure. in STP 1343 Advances in Fatigue Crack Closure Measurement and Analysis: Second Volume 41–56 54 Riemelmoser, F. O. and Pippan, R. (1997) Crack closure: a concept of fatigue crack growth under examination. Fatigue and Fracture of Engineering Materials and Structures, 20, 1529–1540. 55 Dugdale, D. S. (1960) Yielding of steel sheets containing slits. Journal of the Mechanics and Physics of Solids, 8, 100–104. 56 Budiansky, B. and Hutchinson, J. W. (1978) Analysis of closure in fatigue crack growth. Journal of Applied Mechanics, 45, 267–276. 57 Führing, H. and Seeger, T. (1979) Dugdale crack closure analysis of fatigue cracks under constant amplitude loading. Engineering Fracture Mechanics, 11, 99–122. 58 Newman, J. C. (ASTM International, 1981). A crack-closure model for predicting fatigue crack growth under aircraft spectrum loading. in STP 748 Methods and models for predicting fatigue crack growth under random loading 59 de Koning, A. U. and Liefting, G. (ASTM International, 1988). Analysis of crack opening behavior by application of a discretized strip yield model. in STP 982 Mechanics of fatigue crack closure 437–458 60 Sehitoglu, H. (1985) Crack opening and closure in fatigue. Engineering Fracture Mechanics, 21, 329–339. 61 Vormwald, M. and Seeger, T. (1991) The consequences of short crack closure on fatigue crack growth under variable amplitude loading. Fatigue and Fracture of Engineering Materials and Structures, 14, 205–225. 62 Newman, J. C. (ASTM International, 1999). An evaluation of plasticity-induced crack closure concept and measurement methods. in STP 1343 Advances in Fatigue Crack Closure Measurement and Analysis: Second Volume (eds. McClung, R. C. & Newman, J. C.) 128–144 63 McEvily, A. J. (1998). Private Communications. 64 Oberdorfer, B., Setman, D., Steyskal, E. M., Hohenwarter, A., Sprengel, W., Zehetbauer, M., Pippan, R. and Würschum, R. (2014) Grain boundary excess volume and defect annealing of copper after high-pressure torsion. Acta Materialia, 68, 189–195. 65 Fischlschweiger, M., Ecker, W. and Pippan, R. (2012) Veriﬁcation of a continuum mechanical explanation of plasticityinduced crack closure under plain strain conditions by means of ﬁnite element analysis. Engineering Fracture Mechanics, 96, 762–765. 66 Zhou, X., Gaenser, H.-P. and Pippan, R. (2016) The effect of single overloads in tension and compression on the fatigue crack propagation behaviour of short cracks. International Journal of Fatigue, 89, 77–86. 67 Benz, C. and Sander, M. (2015) Reconsiderations of fatigue crack growth at negative stress ratios: ﬁnite element analyses. Engineering Fracture Mechanics, 145, 98–114.

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

FATIGUE CRACK CLOSURE

68 Pippan, R. (1991) Threshold and effective threshold of fatigue crack propagation in ARMCO iron I: the inﬂuence of grain size and cold working. Materials Science and Engineering A, 138, 1–13. 69 Pippan, R., Strobl, G., Kreuzer, H. and Motz, C. (2004) Asymmetric crack wake plasticity – a reason for roughness induced crack closure. Acta Materialia, 52, 4493–4502. 70 Suresh, S. and Ritchie, R. O. (1983) Near-threshold fatigue crack propagation: a perspective on the role of crack closure. J. Me, 35, A4–A4. 71 Wasen, J., Hamberg, K. and Karlsson, B. (1988) The inﬂuence of grain size and fracture surface geometry on the nearthreshold fatigue crack growth in ferritic steels. Materials Science and Engineering A, 102, 217–226. 72 Zerbst, U., Vormwald, M., Pippan, R., Gänser, H.-P., Sarrazin-Baudoux, C. and Madia, M. (2016) About the fatigue crack propagation threshold of metals as a design criterion – a review. Engineering Fracture Mechanics, 153, 190–243. 73 Leitner, T., Hohenwarter, A. and Pippan, R. (2015) Revisiting fatigue crack growth in various grain size regimes of Ni. Materials Science and Engineering A, 646, 294–305. 74 Pokluda, J. and Pippan, R. (2007) Analysis of roughnessinduced crack closure based on asymmetric crack-wake plasticity and size ratio effect. Materials Science and Engineering A, 462, 355–358. 75 Pippan, R., Kolednik, O. and Lang, M. (1994) Mechanism for plasticity-induced crack closure under plane strain conditions. Fatigue and Fracture of Engineering Materials and Structures, 17, 721–726. 76 Cadman, A. J., Brook, R. and Nicholson, C. E. (1983) Factors affecting the measurement of the fatigue threshold (ΔKth). Scripta Metallurgica, 17, 1053–1056. 77 Tabernig, B. and Pippan, R. (2002) Determination of the length dependence of the threshold for fatigue crack propagation. Engineering Fracture Mechanics, 69, 899–907. 78 Hertzberg, R. W., Newton, C. H. and Jaccard, R. (ASTM International, 1988). Crack closure: correlation and confusion. in STP 982 Mechanics of fatigue crack closure 35–43 79 Anderson, T. L. (2005) Fracture Mechanics: Fundamentals and Applications, CRC press: Boca Raton. 80 Shih, C. F. (1981) Relationships between the J-integral and the crack opening displacement for stationary and extending cracks. Journal of the Mechanics and Physics of Solids, 29, 305–326. 81 Riemelmoser, F. O., Gumbsch, P. and Pippan, R. (2001) Dislocation modelling of fatigue cracks: an overview. Materials Transactions, 42, 2–13. 82 Riemelmoser, F. O. and Pippan, R. (ASTM International, 1999). On the ΔKeff concept: an investigation by means of a discrete dislocation model. in STP 1343 Advances in Fatigue Crack Closure Measurement and Analysis: Second Volume 83 Gilbert, C. J., McNaney, J. M., Dauskardt, R. H. and Ritchie, R. O. (1994) Back-face strain compliance and electricalpotential crack length calibrations for the disk-shaped compact-tension DC (T) specimen. Journal of Testing and Evaluation, 22, 117–120. 84 Bray, G. H. and Donald, J. K. (ASTM International, 1999). in STP 1343 advances in fatigue crack closure measurement and analysis: second volume 85 Jono, M., Sugeta, A. and Uematsu, Y. (ASTM International, 1999). Fatigue crack growth and crack closure behavior of Ti-6Al-4 V alloy under variable-amplitude loadings. in STP 1343 Advances in Fatigue Crack Closure Measurement and Analysis: Second Volume (eds. McClung, R. C. & Newman, J. C.) 265–284

493

86 Pippan, R. (1988) The sensitivity to measure crack closure with strain gauges near the crack tip. Engineering Fracture Mechanics, 31, 867–871. 87 Larsen, J. M., Thompson, A. W. and Williams, J. C. (1985) Growth of small cracks in Ti-Al alloys. J. Met., 37, A65–A65. 88 Troha, W. A., Nicholas, T. and Grandt, A. F. (ASTM International, 1988). Three-dimensional aspects of fatigue crack closure in surface ﬂaws in polymethylmethacrylate material. in STP 982 Mechanics of Fatigue Crack Closure 89 Ray, S. K. and Grandt, A. F. (ASTM International, 1988). Comparison of methods for measuring fatigue crack closure in a thick specimen. in STP 982 Mechanics of Fatigue Crack Closure 90 Nowell, D., Paynter, R. J. H. and DE MATOS, P. F. P. (2010) Optical methods for measurement of fatigue crack closure: moiré interferometry and digital image correlation. Fatigue and Fracture of Engineering Materials and Structures, 33, 778–790. 91 Pippan, R. and Grosinger, W. (2013) Fatigue crack closure: from LCF to small scale yielding. International Journal of Fatigue, 46, 41–48. 92 McClung, R. C. and Davidson, D. L. (ASTM International, 1999). Near-tip and remote characterization of plasticityinduced fatigue crack closure. in STP 1343 Advances in Fatigue Crack Closure Measurement and Analysis: Second Volume (eds. McClung, R. C. & Newman, J. C.) 106–127 93 Riddell, W. T., Piascik, R. S., Sutton, M. A., Zhao, W., McNeill, S. R. and Helm, J. D. (ASTM International, 1999). Determining fatigue crack opening loads from near-crack-tip displacement measurements. in STP 1343 Advances in Fatigue Crack Closure Measurement and Analysis: Second Volume (eds. McClung, R. C. & Newman, J. C.) 157–174 94 Sutton, M. A., Zhao, W., McNeill, S. R., Helm, J. D., Piascik, R. S. and Riddell, W. T. (ASTM International, 1999). Local crack closure measurements: development of a measurement system using computer vision and a far-ﬁeld microscope. in STP 1343 Advances in Fatigue Crack Closure Measurement and Analysis: Second Volume (eds. McClung, R. C. & Newman, J. C.) 145–156 95 Maire, E. and Withers, P. J. (2014) Quantitative X-ray tomography. International Materials Review, 59, 1–43. 96 Steuwer, A., Edwards, L., Pratihar, S., Ganguly, S., Peel, M., Fitzpatrick, M. E., Marrow, T. J., Withers, P. J., Sinclair, I., Singh, K. D., Gao, N., Buslaps, T. and Bufﬁère, J.-Y. (2006) In situ analysis of cracks in structural materials using synchrotron X-ray tomography and diffraction. Nucl. Instruments Methods Phys. Res. Sect. B Beam Interact. Mater. Atoms, 246, 217–225. 97 Lopez-Crespo, P., Mostafavi, M., Steuwer, A., Kelleher, J. F., Buslaps, T. and Withers, P. J. (2016) Characterisation of overloads in fatigue by 2D strain mapping at the surface and in the bulk. Fatigue and Fracture of Engineering Materials and Structures, 39, 1040–1048. 98 Döker, H. and Bachmann, V. (ASTM International, 1988). Determination of crack opening load by use of threshold behavior. in Mechanics of fatigue crack closure (eds. Newman, J. C. & Elber, W.) 247–259 99 Bichler, C. and Pippan, R. (2007) Effect of single overloads in ductile metals: a reconsideration. Engineering Fracture Mechanics, 74, 1344–1359. 100 Solanki, K., Daniewicz, S. R. and Newman, J. C. (2004) Finite element analysis of plasticity-induced fatigue crack closure: an overview. Engineering Fracture Mechanics, 71, 149–171.

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

494

R. PIPPAN AND A. HOHENWARTER

101 Buck, O., Thompson, R. B. and Rehbein, D. K. (1988) Ultrasonic measurements of crack tip shielding by closure. Materials Science and Engineering A, 103, 37–42. 102 Pippan, R., Haas, G. and Stüwe, H. P. (1989) Comparison of two methods to measure crack closure in ultra-high vacuum. Engineering Fracture Mechanics, 34, 1075–1084. 103 Newman, J. C. (ASTM International, 1976). A ﬁnite-element analysis of fatigue crack closure. in STP 590 Mechanics of Crack Growth 281–301 104 Chermahini, R. G., Shivakumar, K. N., Newman, J. C. and Blom, A. F. (1989) Three-dimensional aspects of plasticityinduced fatigue crack closure. Engineering Fracture Mechanics, 34, 393–401. 105 Chermahini, R. G., Palmberg, B. and Blom, A. F. (1993) Fatigue crack growth and closure behaviour of semicircular and semi-elliptical surface ﬂaws. International Journal of Fatigue, 15, 259–263. 106 Roychowdhury, S. and Dodds, R. H. (2003) A numerical investigation of 3-D small-scale yielding fatigue crack growth. Engineering Fracture Mechanics, 70, 2363–2383. 107 Roychowdhury, S. and Dodds, R. H. (2005) Effects of an overload event on crack closure in 3-D small-scale yielding: ﬁnite element studies. Fatigue and Fracture of Engineering Materials and Structures, 28, 891–907. 108 Wei, L.-W. and James, M. N. (2002) Fatigue crack closure for inclined and kinked cracks. International Journal of Fracture, 116, 25–50. 109 Suresh, S. and Ritchie, R. O. (1983) Some considerations on the modelling of oxide-induced fatigue crack closure using solutions for a rigid wedge inside a linear elastic crack. Scripta Metallurgica, 17, 575–580. 110 McClung, R. C. and Davidson, D. L. (1991) High resolution numerical and experimental studies of fatigue cracks. Engineering Fracture Mechanics, 39, 113–130. 111 McClung, R. C. and Sehitoglu, H. (1989) On the ﬁnite element analysis of fatigue crack closure – 1. Basic modeling issues. Engineering Fracture Mechanics, 33, 237–252. 112 McClung, R. C., Thacker, B. H. and Roy, S. (1991) Finite element visualization of fatigue crack closure in plane stress and plane strain. International Journal of Fracture, 50, 27–49. 113 Sander, M. and Richard, H. A. (2006) Fatigue crack growth under variable amplitude loading part II: analytical and numerical investigations. Fatigue and Fracture of Engineering Materials and Structures, 29, 303–319. 114 Llorca, J. and Sànchez Gàlvez, V. (1990) Modelling plasticityinduced fatigue crack closure. Engineering Fracture Mechanics, 37, 185–196. 115 Fleck, N. A. (1986) Finite element analysis of plasticityinduced crack closure under plane strain conditions. Engineering Fracture Mechanics, 25, 441–449. 116 Tvergaard, V. (2006) Effect of underloads or overloads in fatigue crack growth by crack-tip blunting. Engineering Fracture Mechanics, 73, 869–879. 117 Blom, A. F. and Holm, D. K. (1985) An experimental and numerical study of crack closure. Engineering Fracture Mechanics, 22, 997–1011. 118 Pommier, S. and Bompard, P. (2000) Bauschinger effect of alloys and plasticity-induced crack closure: a ﬁnite element analysis. Fatigue and Fracture of Engineering Materials and Structures, 23, 129–139. 119 Rodrigues, D. M. and Antunes, F. V. (2009) Finite element simulation of plasticity induced crack closure with different

120

121

122

123

124 125

126

127 128

129

130

131

132

133

134

135 136

137

138

material constitutive models. Engineering Fracture Mechanics, 76, 1215–1230. Sehitoglu, H., Gall, K. and García, A. M. (1996) Recent advances in fatigue crack growth modeling. International Journal of Fracture, 80, 165–192. Jiang, Y. and Feng, M. (2004) Modeling of fatigue crack propagation. Journal of Engineering Materials and Technology, 126, 77–86. Hudak, S. J. and Davidson, D. L. (ASTM International, 1988). The dependence of crack closure on fatigue loading variables. in STP 982 Mechanics of Fatigue Crack Closure (eds. Newman, J. C. & Elber, W.) 121–138 Maierhofer, J., Pippan, R. and Gänser, H.-P. (2014) Modiﬁed NASGRO equation for physically short cracks. International Journal of Fatigue, 59, 200–207. Wheeler, O. E. (1972) Spectrum loading and crack growth. Journal of Basic Engineering, 94, 181–186. Skorupa, M. (1998) Load interaction effects during fatigue crack growth under variable amplitude loading – a literature review. Part I: empirical trends. Fatigue and Fracture of Engineering Materials and Structures, 21, 987–1006. Skorupa, M. (1999) Load interaction effects during fatigue crack growth under variable amplitude loading – a literature review. Part II: qualitative interpretation. Fatigue and Fracture of Engineering Materials and Structures, 22, 905–926. Pommier, S. (2002) Plane strain crack closure and cyclic hardening. Engineering Fracture Mechanics, 69, 25–44. Saxena, V. K. and Radhakrishnan, V. M. (1998) Development of fatigue crack closure mechanism maps part 1 – basic concepts and boundary equations. Materials Science and Technology, 14, 1227–1232. Maierhofer, J., Gaenser, H.-P. and Pippan, R. (2014) Process model for introducing residual stresses by deep rolling. Materialwissenschaft und Werkstofftechnik, 45, 982–989. Fischer, F. D., Daves, W., Pippan, R. and Pointner, P. (2006) Some comments on surface cracks in rails. Fatigue and Fracture of Engineering Materials and Structures, 29, 938–948. Predan, J., Pippan, R. and Gubeljak, N. (2010) Fatigue crack propagation in threshold regime under residual stresses. International Journal of Fatigue, 32, 1050–1056. Sadananda, K., Vasudevan, A. K., Holtz, R. L. and Lee, E. U. (1999) Analysis of overload effects and related phenomena. International Journal of Fatigue, 21, S233–S246. Lang, M. (2000) A model for fatigue crack growth, part II: modelling. Fatigue and Fracture of Engineering Materials and Structures, 23, 603–618. Noroozi, A. H., Glinka, G. and Lambert, S. (2008) Prediction of fatigue crack growth under constant amplitude loading and a single overload based on elasto-plastic crack tip stresses and strains. Engineering Fracture Mechanics, 75, 188–206. Suresh, S. and Ritchie, R. O. (1984) Propagation of short fatigue cracks. Int. Met. Rev., 29, 445–477. Pippan, R., Berger, M. and Stüwe, H. P. (1987) The inﬂuence of crack length on fatigue crack growth in deep sharp notches. Metallurgical Transactions A, 18, 429–435. Pippan, R. and Stüwe, H. P. (1986). Fatigue crack growth behaviour in constant-load amplitude and constant delta-K tests on notched specimens. in ECF6, Amsterdam 1986 Tanaka, K. and Nakai, Y. (1984) Prediction of fatigue threshold of notched components. Journal of Engineering Materials and Technology, 106, 192–199.

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495

FATIGUE CRACK CLOSURE

139 Pippan, R., Plöchl, L., Klanner, F. and Stüwe, H. P. (1994) The use of fatigue specimens precracked in compression for measuring threshold values and crack growth. Journal of Testing and Evaluation, 22, 98–103. 140 Benz, C. and Sander, M. (2014). Fatigue crack growth testing at negative stress ratios : discussion on the comparability of testing results. Fatigue and Fracture of Engineering Materials and Structures, 37, 62–71.

495

141 Yu, M. T. and Topper, T. H. (1985) The effects of Material strength, stress ratio, and compressive overload on the threshold behavior of a SAE1045 Steel. Journal of Engineering Materials and Technology, 107, 19–25. 142 Dowling, N. E. and Iyyer, N. S. (1987) Fatigue crack growth and closure at high cyclic strains. Materials Science and Engineering, 96, 99–107.

© 2017 The Authors Fatigue & Fracture of Engineering Materials & Structures Published by John Wiley & Sons Ltd. Fatigue Fract Engng Mater Struct, 2017, 40, 471–495